www.inframet.pl email: [email protected] INFRAMET tel: 048 608445873, fax 48 22 6668780

2.4 Radiant properties of materials

Radiant properties of a material describe its ability to emit, absorb, reflect and transmit optical radiation. Terminology of radiant properties of materials is probably one the most confusing areas of technical terminology. Authors of different publications use different and sometimes inconsistent definitions. The situation is so complicated that some parameters used in literature to describe material ability to emit, absorb, reflect and transmit radiation were not included in the well known terminology standard of optical radiation - the International Lighting Vocabulary [1] - as the CIE decided that further work was needed to establish proper names and definitions of some parameters; particularly describing material ability to reflect and transmit radiation. Next, although the ILV can be considered as the most important terminology standard, there are other standards or books [4,5,6] that propose solutions that differ from the ones found in the ILV. Further on, even the authors [7] that generally accepted the terminology proposed in the IVL add their own exceptions. And finally there are publications that use terminology that is inconsistent width both with the ILV or the works [4,5,6]. According to a school of terminology proposed in work [2] the words used to describe the various radiometric properties of materials should have very specific meaning; especially their endings. In this way, any word that ends in ion describes a process: emission, absorption, reflection, transmission. Any words that ends in ance represents a property of a specific sample. Finally, any words that ends in ivity represents a property of the generic material. The International Lighting Vocabulary of the CIE generally follows this school of thought and proposes following parameters: reflectance and reflectivity, absorptance and absorptivity, transmittance and transmissivity to describe property of a specific sample or a property of the generic material. Reflectance (for incident radiation of a given spectral composition, polarization and geometrical distribution) (ρ) is defined in the ILV as a ratio of the reflected flux to the incident flux in the given conditions. Reflectivity (of a material) (ρ∝ ) is reflectance of a layer of the material of such a thickness that there is no change of reflectance with increase in thickness. Absorptance (α) is defined as ratio of the flux absorbed by the material to flux incident on it under specified conditions. Spectral absorptivity (of an absorbing material) αi,o(λ) is spectral internal absorptance of a layer of the material such that the path of the radiation is of unit length, and under the conditions in which the boundary of the material has no influence. Transmittance (for incident radiation of a given spectral composition, polarization and geometrical distribution) (τ) is ratio of the transmitted flux to the incident flux in the given conditions. Spectral transmissivity (of an absorbing material) τi,o(λ) is spectral internal transmittance of a layer of the material such that the path of the radiation is of unit length, and under the conditions in which the boundary of the material has no influence. As pointed by Siegel and Howell [4] for substances opaque at the wavelengths of emission, the intrinsic and the extrinsic parameters describing material ability to emit radiation would be the same as the emission of radiant flux from a opaque material is a surface phenomenon. Probably because of this reason the ILV uses only one term "the emissivity" and symbol ε to describe emissive properties of non-blackbodies surfaces. However, the 1993 Handbook of Fundamentals of the American Society of Heating , Refrigerating, and Air- Conditioning Engineers [5] uses term "emittance" and the symbol ε to describe emissive properties of actual pieces of materials and points that the term emissivity refers to the property of materials that are optically smooth and thick enough

PROPRIETARY INFORMATION: No portion of this document can be reproduced, copied, exhibited or otherwise used without specific written authorisation from INFRAMET. www.inframet.pl email: [email protected] INFRAMET tel: 048 608445873, fax 48 22 6668780 to be opaque. A relatively new American Society for Testing of Materials (ASTM) standard [6] follows this terminology but uses the Roman letter e for emittance and the Greek letter ε for emissivity. Next, there are publications [3] that use the terms "emittance" to mean flux density (an equivalent of earlier defined exitance), not as a mean of radiation efficiency. Further on, there exist publications [8,11] where the terms "absorptivity", "reflectivity" and "transmissivity" have meanings of the terms "absorptance", "reflectance" and "transmittance" defined according to earlier presented scheme. Finally, the term "transmission" is used in the Handbook of Infrared &Electro-Optical Systems of SPIE [9] as a quantity describing material property in situation when according to the mentioned earlier standards [1,5,6] this terms is restricted to describe the process. We will keep to the recommendation of the ILV through the remainder of this book and use the terms "emissivity", "absorptance", "reflectance" and "transmittance" to describe properties of a specific sample. However, a reader must be aware that this school of terminology is not universally accepted. For people carrying out not-contact temperature measurements material ability to emit radiation is the most important material property. Therefore, in this subchapter we will concentrate on different kinds of the term “emissivity1” used in literature to describe material ability to emit radiation and relationships between emissivity, absorptance, reflectance and transmittance. Because of the mentioned earlier confusion in terminology only these types of emissivity, absorptance, reflectance and transmittance really needed to explain principles of non-contact temperature measurement will be defined next. This limitation is really important as at least eight types of emissivity, four types of absorptance, eight types of reflectance and eight types of transmittance are used in literature to describe material ability to absorb, reflect and transmit radiation.

Emission properties A blackbody is an ideal radiator which emits as much radiant energy as possible. Such emission can occur only inside an isothermal closed cavity. It is not possible to observe emission of this completely closed cavity. However, it is possible to manufacture a technical blackbody made as a cavity with a small hole in one of the cavity walls. Emission of such a technical blackbody is very close to that of an ideal blackbody. Emission of real materials is lower that that of an ideal blackbody and we need parameters to characterize the emissive properties of such real materials. The properties are defined by comparison with that of blackbodies at the same temperature and can be described by four parameters: spectral directional emissivity, spectral (hemispherical) emissivity, directional (total) emissivity and total 2 (hemispherical) emissivity [8,11].

The spectral directional emissivity ελ,ϕ depends on the wavelength λ and the angle ϕ and is defined as in the formula L ε = λ,ϕ λ,ϕ L λ ϕ bb, , (2.16) where Lλ,ϕ is the spectral radiance of the material for the wavelength λ in the direction ϕ and Lbb,λ,ϕ is the spectral radiance of the blackbody for the wavelength λ in the direction ϕ.

1 Only two kinds of emissivity (directional emissivity and hemispherical emissivity) are defined in the ILV. 2 The adjectives in brackets are usually not mentioned. PROPRIETARY INFORMATION: No portion of this document can be reproduced, copied, exhibited or otherwise used without specific written authorisation from INFRAMET. www.inframet.pl email: [email protected] INFRAMET tel: 048 608445873, fax 48 22 6668780

A particular kind of the spectral emissivity in the direction ϕ occurs for ϕ=0; in the direction normal to the radiating surface as the value of the spectral emissivity is the greatest in this direction. The spectral emissivity in the normal direction ελ,n can be expressed by the formula L ε = λ,n λ,ϕ (2.17) Lbb,λ,n where Lλ,n is the spectral radiance of material in the normal direction, and Lbb,λ,n is the spectral radiance of the blackbody in normal direction. On account of the needs of visual pyrometry, values of normal spectral emissivity for red light are often presented in many emissivity tables [11]. This quantity is expressed by ελ=0.65,n, where 0.65 is the wavelength in µm. The spectral (hemispherical) emissivity ελ is defined as ratio of the material spectral exitance Mλ to the blackbody spectral exitance Mbb,λ

M λ,n ελ = . (2.18) M bb,λ,n

Directional (total) emissivity in the direction ϕ is expressed as ratio of the material radiance LT,ϕ in the direction ϕ to the blackbody radiance LT,ϕ in the direction ϕ L ε = T ,ϕ T ,ϕ . (2.19) Lbb,T ,ϕ

Directional total emissivity in the normal direction εT,n is a particularly privileged kind of directional total emissivity εT,ϕ for the same reasons as the spectral emissivity in normal direction ελ,n. It can be expressed by the formula L ε = T ,n T ,n . (2.20) Lbb,T ,n where LT,n is the material radiance in the normal direction, and Lbb,T,n is the blackbody radiance in normal direction. This type of emissivity is most frequently measured and quoted in literature. It is often confused with the spectral (hemispherical) emissivity ελ.

Finally, the total hemispherical emissivity εT is defined as ratio of the material exitance MT to the blackbody exitance Mbb,T

ε = MT T . (2.21) M bb,T

The spectral directional emissivity ελ,ϕ gives information about material emissive properties for any the wavelength λ and the angle ϕ. On the basis of the known spectral directional emissivity

ελ,ϕ it is possible to calculate other types of emissivity: the spectral (hemispherical) emissivity ελ, the directional total emissivity εT,n and the total hemispherical emissivity εT. However, as the spectral directional emissivity ελ,ϕ is often a complex function of the wavelength λ and the angle ϕ it is difficult to determine it experimentally. Therefore, functions of the spectral directional emissivity ελ,ϕ are very rarely published in literature. There are four types of emissivity that are usually presented in emissivity tables found in literature: the total hemispherical emissivity εT, the directional total emissivity in normal direction εT,n, the spectral directional emissivity in normal direction ελ,n and spectral directional emissivity in the

PROPRIETARY INFORMATION: No portion of this document can be reproduced, copied, exhibited or otherwise used without specific written authorisation from INFRAMET. www.inframet.pl email: [email protected] INFRAMET tel: 048 608445873, fax 48 22 6668780

normal direction ελ=0.65,n for wavelength λ=0.65µm. However, their usefulness for user of modern non- contact radiation thermometers is usually limited because of a few reasons.

First, the total emissivity εT gives information about material emission into whole hemisphere and in whole optical range. Therefore, values of the εT are useful only in case of diffusive gray-body types objects, emissive properties of which do not depend on the angle ϕ and the wavelength λ.

Second, directional total emissivity in the normal direction εT,n presents information about material ability to emit radiation only into one direction (ϕ = 0) and in whole range of optical radiation. The angle ϕ often differs from 0 during real measurements. As emissive properties of most material depend on the angle of observation ϕ the value of the εT,n can be misleading. There is also other reason for limited usefulness of the directional total emissivity in the normal direction εT,n. Most real materials are selective materials, emissive properties of which depend on wavelength in situation when sensitivity of most non-contact thermometers depend on wavelength, too.

Third, the spectral directional emissivity in the normal direction ελ,n presents information about material ability to emit radiation into only one direction (ϕ = 0). Therefore, the values of ελ,n can be misleading when measurements are done for other angles. In spite of this, the published functions ελ,n (λ) are usually quite useful as they enable estimation of object emissivity in the thermometer spectral band. However, there is often a problem to find suitable data of ελ,n in the required spectral band.

Fourth, values of spectral directional emissivity in the normal direction ελ=0.65,n for the wavelength

λ=0.65µm are often useless in case of typical infrared systems as the spectral emissivity ελ,n in infrared range can differ quite significantly from ελ=0.65,n.

Relationships between radiative properties of materials There are two most important relationships between radiative properties of materials. The first is the radiative energy balance that connects absorptance, reflectance and transmittance. The second is Kirchhoff's law that relates absorptance and emissivity. Applying energy balance on the surface element, we get that that the sum of hemispherical total absorptance αT, the hemispherical total reflectance ρT and the hemispherical total transmittance τT equals 1

αT +ρT +τT =1 (2.22) Next, assuming elementary spectral interval and that some phenomena (luminescence, Raman scattering) are negligible we can write

αλ +ρλ +τλ =1 (2.23) where αλ is the hemispherical spectral absorptance of radiation from the hemisphere, ρλ is the hemispherical spectral reflectance of radiation from hemisphere into hemisphere, and τλ is hemispherical spectral transmittance of radiation from hemisphere into hemisphere. Radiation that reaches material surface comes often not from the whole hemisphere but only from a certain direction. For such a situation the relationships between directional quantities that can be treated as directional spectral energy balance can be written as

αλ,ϕ +ρλ, ϕ +τλ,ϕ =1 (2.24) where αλ,ϕ is the directional spectral absorptance of radiation from the direction ϕ, ρλ,ϕ is directional- hemispherical spectral reflectance of radiation from the direction ϕ into hemisphere, and τλ,ϕ is the directional-hemispherical spectral transmittance. The Kirchhoff's law states that at local thermodynamic equilibrium of an element of material surface, that the directional spectral emissivity ελ,ϕ is equal to the directional spectral absorptance αλ,ϕ

PROPRIETARY INFORMATION: No portion of this document can be reproduced, copied, exhibited or otherwise used without specific written authorisation from INFRAMET. www.inframet.pl email: [email protected] INFRAMET tel: 048 608445873, fax 48 22 6668780

ελ,ϕ = αλ,ϕ (2.25) It means that material ability to emit radiation into the direction ϕ is directly connected to its ability to absorb radiation from the direction ϕ .

Formulas (2.24, 2.25) enable indirect determination of the directional spectral emissivity ελ,ϕ when the directional-hemispherical spectral reflectance ρλ,ϕ and the directional-hemispherical spectral transmittance τλ,ϕ are known

ελ,ϕ =1- ρλ, ϕ - τλ,ϕ . (2.26) For opaque materials the above presented relationship can be transformed to a new form

ελ,ϕ =1- ρλ, ϕ . (2.27) Principle of temperature measurement with active systems is based on equations (2.26, 2.27) as they enable indirect way of emissivity determination by measuring relations between the incident flux, the reflected flux and the transmitted flux. However, it must be emphasized that to determine ελ,ϕ accurately it is necessary to measure not the radiation reflected into the direction ϕ but into the hemisphere. This misconception brought significant errors in great number of measurements.

Emissivity of common materials Tables or graphs with data about the four types of emissivity (the total hemispherical emissivity εT, directional total emissivity in the normal direction εT,n, the spectral directional emissivity in normal direction ελ,n and spectral directional emissivity in the normal direction ελ=0.65,n for wavelength λ=0.65µm) can be found in great number of books, papers, reports etc. However, in addition to the discussed in Section 2.4.1 limitations of these parameters there are additional problem with interpretation of typical emissivity data found in literature. First, different sources present sometimes completely inconsistent values. Second, emissivity values are often unclearly defined or they are not defined at all. Parameters in many tables are termed only “emissivity” without any additional explanation whether it is the total hemispherical emissivity εT, directional total emissivity in the normal direction εT,n or spectral directional emissivity in the normal direction ελ=0.65,n for the wavelength λ=0.65µm. As an example can be treated Tab. 2.5 and Tab. 2.6 with emissivities of common materials published by one of leading manufacturers of thermal cameras [12]. The manufacturer, however, honestly emphasizes that the presented values are meant to be used only as a guide and can vary depending on many different factors. To summarize, we can say that in spite of numerous sources with emissivity data it is often difficult to find in literature information about value of object emissivity in real measurement conditions.

PROPRIETARY INFORMATION: No portion of this document can be reproduced, copied, exhibited or otherwise used without specific written authorisation from INFRAMET. www.inframet.pl email: [email protected] INFRAMET tel: 048 608445873, fax 48 22 6668780

Tab. 2.5. Typical emissivities of common metals Material Temperature Emissivity [°C] Aluminum: foil (bright) 20 0.04 weathered 20 0.83 - 0.94 Iron cast, oxidized 100 0.64 sheet, heavily rusted 20 0.69 - 0.96 Copper: polished 100 0.05 heavily oxidized 0.78 0.78 Nickel: electroplated, polished 20 0.05 Stainless Steel polished 20 0.16 (type 18-8) oxidized 60 0.85 Steel polished 100 0.07 oxidized 200 0.79

Tab. 2.6. Typical emissivities of other materials Other materials: Brick common red 20 0.93 Carbon candle soot 20 0.95 Concrete dry 35 0.95 Glass chemical ware 35 0.95 Oil lubricating 17 0.87 film thickness 0.03 mm 20 0.27 film thickness 0.13 mm 20 0.72 thick coating 20 0.82 Paint, oil average of 16 colors 20 0.94 Paper white 20 0.7 - 0.90 Plaster 20 0.86 - 0.90 Rubber black 5 20 0.95 Skin human 32 0.98 Soil dry 20 0.92 saturated with water 20 0.95 Water distilled 20 0.96 frost crystals -10 0.98 snow -10 0.85 Wood planed oak 20 0.90

PROPRIETARY INFORMATION: No portion of this document can be reproduced, copied, exhibited or otherwise used without specific written authorisation from INFRAMET.